DOI: 10.17188/1684262
title: Materials Data on Na7(WO3)20 by Materials Project

description: Na7(WO3)20 crystallizes in the tetragonal P4mm space group. The structure is three-dimensional. there are seven inequivalent Na sites. In the first Na site, Na is bonded to twelve O atoms to form NaO12 cuboctahedra that share corners with four equivalent NaO12 cuboctahedra, faces with four equivalent NaO12 cuboctahedra, and faces with eight WO6 octahedra. There are a spread of Na–O bond distances ranging from 2.71–2.75 Å. In the second Na site, Na is bonded to twelve O atoms to form NaO12 cuboctahedra that share corners with four equivalent NaO12 cuboctahedra, faces with four equivalent NaO12 cuboctahedra, and faces with eight WO6 octahedra. There are a spread of Na–O bond distances ranging from 2.71–2.75 Å. In the third Na site, Na is bonded to twelve O atoms to form NaO12 cuboctahedra that share corners with eight NaO12 cuboctahedra, faces with five NaO12 cuboctahedra, and faces with eight WO6 octahedra. There are a spread of Na–O bond distances ranging from 2.69–2.80 Å. In the fourth Na site, Na is bonded to twelve O atoms to form NaO12 cuboctahedra that share corners with eight NaO12 cuboctahedra, faces with five NaO12 cuboctahedra, and faces with eight WO6 octahedra. There are a spread of Na–O bond distances ranging from 2.68–2.78 Å. In the fifth Na site, Na is bonded to twelve O atoms to form NaO12 cuboctahedra that share corners with eight NaO12 cuboctahedra, faces with five NaO12 cuboctahedra, and faces with eight WO6 octahedra. There are a spread of Na–O bond distances ranging from 2.67–2.81 Å. In the sixth Na site, Na is bonded to twelve O atoms to form NaO12 cuboctahedra that share corners with twelve NaO12 cuboctahedra, faces with six NaO12 cuboctahedra, and faces with eight WO6 octahedra. There are a spread of Na–O bond distances ranging from 2.73–2.78 Å. In the seventh Na site, Na is bonded to twelve O atoms to form NaO12 cuboctahedra that share corners with eight NaO12 cuboctahedra, faces with five NaO12 cuboctahedra, and faces with eight WO6 octahedra. There are a spread of Na–O bond distances ranging from 2.70–2.82 Å. There are twenty inequivalent W sites. In the first W site, W is bonded to six O atoms to form WO6 octahedra that share corners with six WO6 octahedra and faces with four equivalent NaO12 cuboctahedra. The corner-sharing octahedra tilt angles range from 0–3°. There are a spread of W–O bond distances ranging from 1.93–1.98 Å. In the second W site, W is bonded to six O atoms to form WO6 octahedra that share corners with six WO6 octahedra and faces with four equivalent NaO12 cuboctahedra. The corner-sharing octahedra tilt angles range from 0–9°. There are a spread of W–O bond distances ranging from 1.84–2.04 Å. In the third W site, W is bonded to six O atoms to form corner-sharing WO6 octahedra. The corner-sharing octahedra tilt angles range from 0–7°. There are a spread of W–O bond distances ranging from 1.85–2.08 Å. In the fourth W site, W is bonded to six O atoms to form corner-sharing WO6 octahedra. The corner-sharing octahedra tilt angles range from 0–6°. There are a spread of W–O bond distances ranging from 1.86–2.05 Å. In the fifth W site, W is bonded to six O atoms to form corner-sharing WO6 octahedra. The corner-sharing octahedra tilt angles range from 0–5°. There are a spread of W–O bond distances ranging from 1.88–2.03 Å. In the sixth W site, W is bonded to six O atoms to form corner-sharing WO6 octahedra. The corner-sharing octahedral tilt angles are 0°. There is four shorter (1.95 Å) and two longer (1.96 Å) W–O bond length. In the seventh W site, W is bonded to six O atoms to form corner-sharing WO6 octahedra. The corner-sharing octahedra tilt angles range from 0–3°. There are a spread of W–O bond distances ranging from 1.91–2.00 Å. In the eighth W site, W is bonded to six O atoms to form corner-sharing WO6 octahedra. The corner-sharing octahedra tilt angles range from 0–5°. There are a spread of W–O bond distances ranging from 1.88–2.03 Å. In the ninth W site, W is bonded to six O atoms to form corner-sharing WO6 octahedra. The corner-sharing octahedra tilt angles range from 0–3°. There are a spread of W–O bond distances ranging from 1.92–2.00 Å. In the tenth W site, W is bonded to six O atoms to form corner-sharing WO6 octahedra. The corner-sharing octahedra tilt angles range from 0–8°. There are a spread of W–O bond distances ranging from 1.84–2.08 Å. In the eleventh W site, W is bonded to six O atoms to form corner-sharing WO6 octahedra. The corner-sharing octahedra tilt angles range from 0–6°. There are a spread of W–O bond distances ranging from 1.86–2.05 Å. In the twelfth W site, W is bonded to six O atoms to form WO6 octahedra that share corners with six WO6 octahedra and faces with four equivalent NaO12 cuboctahedra. The corner-sharing octahedra tilt angles range from 0–5°. There are a spread of W–O bond distances ranging from 1.89–1.98 Å. In the thirteenth W site, W is bonded to six O atoms to form WO6 octahedra that share corners with six WO6 octahedra and faces with four equivalent NaO12 cuboctahedra. The corner-sharing octahedra tilt angles range from 0–10°. There are a spread of W–O bond distances ranging from 1.84–2.05 Å. In the fourteenth W site, W is bonded to six O atoms to form WO6 octahedra that share corners with six WO6 octahedra and faces with eight NaO12 cuboctahedra. The corner-sharing octahedra tilt angles range from 0–1°. There is one shorter (1.91 Å) and five longer (1.95 Å) W–O bond length. In the fifteenth W site, W is bonded to six O atoms to form WO6 octahedra that share corners with six WO6 octahedra and faces with four equivalent NaO12 cuboctahedra. The corner-sharing octahedra tilt angles range from 0–6°. There are five shorter (1.95 Å) and one longer (2.06 Å) W–O bond lengths. In the sixteenth W site, W is bonded to six O atoms to form WO6 octahedra that share corners with six WO6 octahedra and faces with four equivalent NaO12 cuboctahedra. The corner-sharing octahedra tilt angles range from 0–7°. There are a spread of W–O bond distances ranging from 1.88–2.03 Å. In the seventeenth W site, W is bonded to six O atoms to form WO6 octahedra that share corners with six WO6 octahedra and faces with eight NaO12 cuboctahedra. The corner-sharing octahedra tilt angles range from 0–1°. There are a spread of W–O bond distances ranging from 1.92–1.95 Å. In the eighteenth W site, W is bonded to six O atoms to form WO6 octahedra that share corners with six WO6 octahedra and faces with four equivalent NaO12 cuboctahedra. The corner-sharing octahedra tilt angles range from 0–7°. There are a spread of W–O bond distances ranging from 1.92–2.03 Å. In the nineteenth W site, W is bonded to six O atoms to form WO6 octahedra that share corners with six WO6 octahedra and faces with eight NaO12 cuboctahedra. The corner-sharing octahedra tilt angles range from 0–2°. There are a spread of W–O bond distances ranging from 1.95–2.02 Å. In the twentieth W site, W is bonded to six O atoms to form WO6 octahedra that share corners with six WO6 octahedra and faces with four equivalent NaO12 cuboctahedra. The corner-sharing octahedra tilt angles range from 0–6°. There are a spread of W–O bond distances ranging from 1.91–2.00 Å. There are forty inequivalent O sites. In the first O site, O is bonded in a distorted rectangular see-saw-like geometry to two equivalent Na and two equivalent W atoms. In the second O site, O is bonded in a distorted rectangular see-saw-like geometry to two equivalent Na and two equivalent W atoms. In the third O site, O is bonded in a linear geometry to two equivalent W atoms. In the fourth O site, O is bonded in a linear geometry to two equivalent W atoms. In the fifth O site, O is bonded in a linear geometry to two equivalent W atoms. In the sixth O site, O is bonded in a linear geometry to two equivalent W atoms. In the seventh O site, O is bonded in a linear geometry to two equivalent W atoms. In the eighth O site, O is bonded in a linear geometry to two equivalent W atoms. In the ninth O site, O is bonded in a linear geometry to two equivalent W atoms. In the tenth O site, O is bonded in a linear geometry to two equivalent W atoms. In the eleventh O site, O is bonded in a linear geometry to two equivalent W atoms. In the twelfth O site, O is bonded in a distorted rectangular see-saw-like geometry to two equivalent Na and two equivalent W atoms. In the thirteenth O site, O is bonded in a distorted rectangular see-saw-like geometry to two equivalent Na and two equivalent W atoms. In the fourteenth O site, O is bonded in a distorted rectangular see-saw-like geometry to two equivalent Na and two equivalent W atoms. In the fifteenth O site, O is bonded to four Na and two equivalent W atoms to form a mixture of distorted edge, face, and corner-sharing ONa4W2 octahedra. The corner-sharing octahedra tilt angles range from 1–62°. In the sixteenth O site, O is bonded in a distorted rectangular see-saw-like geometry to two equivalent Na and two equivalent W atoms. In the seventeenth O site, O is bonded in a distorted rectangular see-saw-like geometry to two equivalent Na and two equivalent W atoms. In the eighteenth O site, O is bonded to four Na and two equivalent W atoms to form a mixture of distorted edge, face, and corner-sharing ONa4W2 octahedra. The corner-sharing octahedra tilt angles range from 1–62°. In the nineteenth O site, O is bonded to four Na and two equivalent W atoms to form a mixture of distorted edge, face, and corner-sharing ONa4W2 octahedra. The corner-sharing octahedra tilt angles range from 1–61°. In the twentieth O site, O is bonded in a linear geometry to two W atoms. In the twenty-first O site, O is bonded to four equivalent Na and two W atoms to form a mixture of distorted edge and corner-sharing ONa4W2 octahedra. The corner-sharing octahedral tilt angles are 0°. In the twenty-second O site, O is bonded in a linear geometry to two W atoms. In the twenty-third O site, O is bonded in a linear geometry to two W atoms. In the twenty-fourth O site, O is bonded in a linear geometry to two W atoms. In the twenty-fifth O site, O is bonded in a linear geometry to two W atoms. In the twenty-sixth O site, O is bonded in a linear geometry to two W atoms. In the twenty-seventh O site, O is bonded in a linear geometry to two W atoms. In the twenty-eighth O site, O is bonded in a linear geometry to two W atoms. In the twenty-ninth O site, O is bonded in a linear geometry to two W atoms. In the thirtieth O site, O is bonded in a linear geometry to two W atoms. In the thirty-first O site, O is bonded in a linear geometry to two W atoms. In the thirty-second O site, O is bonded to four equivalent Na and two W atoms to form a mixture of distorted edge and corner-sharing ONa4W2 octahedra. The corner-sharing octahedral tilt angles are 0°. In the thirty-third O site, O is bonded in a linear geometry to two W atoms. In the thirty-fourth O site, O is bonded to four equivalent Na and two W atoms to form a mixture of distorted edge, face, and corner-sharing ONa4W2 octahedra. The corner-sharing octahedra tilt angles range from 0–62°. In the thirty-fifth O site, O is bonded to four equivalent Na and two W atoms to form a mixture of distorted edge, face, and corner-sharing ONa4W2 octahedra. The corner-sharing octahedra tilt angles range from 0–61°. In the thirty-sixth O site, O is bonded in a linear geometry to two W atoms. In the thirty-seventh O site, O is bonded to four equivalent Na and two W atoms to form a mixture of distorted edge, face, and corner-sharing ONa4W2 octahedra. The corner-sharing octahedra tilt angles range from 0–62°. In the thirty-eighth O site, O is bonded in a distorted rectangular see-saw-like geometry to two equivalent Na and two equivalent W atoms. In the thirty-ninth O site, O is bonded to four equivalent Na and two W atoms to form a mixture of distorted edge, face, and corner-sharing ONa4W2 octahedra. The corner-sharing octahedra tilt angles range from 0–61°. In the fortieth O site,